#------------------------------------------------------------------------------
#$Date: 2021-04-27 12:29:29 +0300 (Tue, 27 Apr 2021) $
#$Revision: 264589 $
#$URL: file:///home/coder/svn-repositories/cod/cif/1/56/21/1562163.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_1562163
loop_
_publ_author_name
'Jin, Geng Bang'
'Soderholm, L.'
_publ_section_title
;
 Solid-state syntheses and single-crystal characterizations of three
 tetravalent thorium and uranium silicates
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              405
_journal_page_last               410
_journal_paper_doi               10.1016/j.jssc.2014.10.018
_journal_volume                  221
_journal_year                    2015
_chemical_formula_moiety         '(Ca0.5 Na0.5)2 Na Th Si8 O20'
_chemical_formula_sum            'Ca Na2 O20 Si8 Th'
_chemical_formula_weight         862.82
_chemical_name_common            'Calcium sodium thorium silicate'
_space_group_IT_number           124
_space_group_name_Hall           '-P 4 2c'
_space_group_name_H-M_alt        'P 4/m c c'
_symmetry_cell_setting           tetragonal
_symmetry_space_group_name_H-M   'P 4/m c c'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            2
_cell_length_a                   7.497(2)
_cell_length_b                   7.497(2)
_cell_length_c                   14.886(4)
_cell_measurement_reflns_used    2491
_cell_measurement_temperature    100(2)
_cell_measurement_theta_max      30.43
_cell_measurement_theta_min      4.72
_cell_volume                     836.7(4)
_computing_cell_refinement       'Bruker APEX2'
_computing_data_collection       'Bruker APEX2'
_computing_data_reduction        'Bruker SAINT'
_computing_molecular_graphics    'CrystalMaker for Windows ver. 2.5.2 (2011)'
_computing_publication_material  'SHELXTL-97 (Sheldrick, 1997)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      100(2)
_diffrn_measured_fraction_theta_full 0.993
_diffrn_measured_fraction_theta_max 0.993
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       '0.3 wide w/ exposures'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0702
_diffrn_reflns_av_sigmaI/netI    0.0260
_diffrn_reflns_limit_h_max       11
_diffrn_reflns_limit_h_min       -11
_diffrn_reflns_limit_k_max       11
_diffrn_reflns_limit_k_min       -11
_diffrn_reflns_limit_l_max       22
_diffrn_reflns_limit_l_min       -22
_diffrn_reflns_number            12468
_diffrn_reflns_theta_full        32.65
_diffrn_reflns_theta_max         32.65
_diffrn_reflns_theta_min         4.72
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    9.958
_exptl_absorpt_correction_T_max  0.727
_exptl_absorpt_correction_T_min  0.706
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   SADABS
_exptl_crystal_colour            colorless
_exptl_crystal_density_diffrn    3.425
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       cube
_exptl_crystal_F_000             808
_exptl_crystal_size_max          0.036
_exptl_crystal_size_mid          0.034
_exptl_crystal_size_min          0.032
_refine_diff_density_max         0.894
_refine_diff_density_min         -0.905
_refine_diff_density_rms         0.212
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.164
_refine_ls_matrix_type           full
_refine_ls_number_parameters     42
_refine_ls_number_reflns         798
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.164
_refine_ls_R_factor_all          0.0349
_refine_ls_R_factor_gt           0.0231
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
; calc 
 [1.00000+0.00000exp(0.00(sinθ/λ)²)]/ 
   [σ²(Fo²)+0.0000+0.0000*P+(0.0289P)²+0.0000sinθ/λ] 
 where P = 1.00000Fo² + 0.00000Fc² 
;
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0510
_refine_ls_wR_factor_ref         0.0563
_reflns_number_gt                642
_reflns_number_total             798
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            JSSC-2015-221-405.cif
_cod_data_source_block           compound2
_cod_depositor_comments
;
The following automatic conversions were performed:

data item '_exptl_crystal_density_meas' value 'not measured' was
changed to '?' -- the value is perceived as not measured.

Automatic conversion script
Id: cif_fix_values 8369 2020-08-20 11:38:08Z andrius 
;
_cod_original_cell_volume        836.6(4)
_cod_database_code               1562163
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, z'
'-y, x, z'
'y, -x, z'
'-x, y, -z+1/2'
'x, -y, -z+1/2'
'y, x, -z+1/2'
'-y, -x, -z+1/2'
'-x, -y, -z'
'x, y, -z'
'y, -x, -z'
'-y, x, -z'
'x, -y, z-1/2'
'-x, y, z-1/2'
'-y, -x, z-1/2'
'y, x, z-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Ca1 Ca 0.0000 0.5000 0.2500 0.0111(3) Uani 0.50 4 d SP . .
Na1 Na 0.0000 0.5000 0.2500 0.0111(3) Uani 0.50 4 d SP . .
Na2 Na 0.0000 0.0000 0.0000 0.079(3) Uani 1 8 d S . .
Th1 Th 0.0000 0.0000 0.2500 0.00838(9) Uani 1 8 d S . .
Si1 Si 0.25735(12) 0.33290(13) 0.10573(6) 0.01036(17) Uani 1 1 d . . .
O1 O 0.1045(3) 0.2485(4) 0.16396(18) 0.0186(5) Uani 1 1 d . . .
O2 O 0.4540(3) 0.2550(4) 0.12875(19) 0.0198(6) Uani 1 1 d . . .
O3 O 0.2204(6) 0.3004(6) 0.0000 0.0296(10) Uani 1 2 d S . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Na Na 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Si Si 0.0817 0.0704 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ca Ca 0.2262 0.3064 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Th Th -7.2400 8.8979 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O1 Ca1 O1 142.05(13) . 6_565
O1 Ca1 O1 77.08(12) . 5
O1 Ca1 O1 115.79(13) 6_565 5
O1 Ca1 O1 115.79(13) . 2_565
O1 Ca1 O1 77.08(12) 6_565 2_565
O1 Ca1 O1 142.05(13) 5 2_565
O1 Ca1 O2 76.76(9) . 3
O1 Ca1 O2 134.25(8) 6_565 3
O1 Ca1 O2 91.47(9) 5 3
O1 Ca1 O2 60.36(8) 2_565 3
O1 Ca1 O2 91.47(9) . 7
O1 Ca1 O2 60.36(8) 6_565 7
O1 Ca1 O2 76.76(9) 5 7
O1 Ca1 O2 134.25(8) 2_565 7
O2 Ca1 O2 165.07(11) 3 7
O1 Ca1 O2 60.36(8) . 4_565
O1 Ca1 O2 91.47(9) 6_565 4_565
O1 Ca1 O2 134.25(8) 5 4_565
O1 Ca1 O2 76.76(9) 2_565 4_565
O2 Ca1 O2 94.21(12) 3 4_565
O2 Ca1 O2 87.73(12) 7 4_565
O1 Ca1 O2 134.25(8) . 8_565
O1 Ca1 O2 76.76(9) 6_565 8_565
O1 Ca1 O2 60.36(8) 5 8_565
O1 Ca1 O2 91.47(9) 2_565 8_565
O2 Ca1 O2 87.73(12) 3 8_565
O2 Ca1 O2 94.21(12) 7 8_565
O2 Ca1 O2 165.07(11) 4_565 8_565
O1 Ca1 Si1 118.34(7) . 6_565
O1 Ca1 Si1 29.15(6) 6_565 6_565
O1 Ca1 Si1 98.51(7) 5 6_565
O1 Ca1 Si1 104.52(6) 2_565 6_565
O2 Ca1 Si1 163.38(6) 3 6_565
O2 Ca1 Si1 31.26(6) 7 6_565
O2 Ca1 Si1 88.33(7) 4_565 6_565
O2 Ca1 Si1 85.74(7) 8_565 6_565
O1 Ca1 Si1 98.51(7) . 2_565
O1 Ca1 Si1 104.52(6) 6_565 2_565
O1 Ca1 Si1 118.34(7) 5 2_565
O1 Ca1 Si1 29.15(6) 2_565 2_565
O2 Ca1 Si1 31.26(6) 3 2_565
O2 Ca1 Si1 163.38(6) 7 2_565
O2 Ca1 Si1 85.74(7) 4_565 2_565
O2 Ca1 Si1 88.33(7) 8_565 2_565
Si1 Ca1 Si1 133.09(4) 6_565 2_565
O1 Ca1 Si1 104.52(6) . 5
O1 Ca1 Si1 98.51(7) 6_565 5
O1 Ca1 Si1 29.15(6) 5 5
O1 Ca1 Si1 118.34(7) 2_565 5
O2 Ca1 Si1 88.33(7) 3 5
O2 Ca1 Si1 85.74(7) 7 5
O2 Ca1 Si1 163.38(6) 4_565 5
O2 Ca1 Si1 31.26(6) 8_565 5
Si1 Ca1 Si1 93.93(4) 6_565 5
Si1 Ca1 Si1 104.38(4) 2_565 5
O1 Ca1 Si1 29.15(6) . .
O1 Ca1 Si1 118.34(7) 6_565 .
O1 Ca1 Si1 104.52(6) 5 .
O1 Ca1 Si1 98.51(7) 2_565 .
O2 Ca1 Si1 85.74(7) 3 .
O2 Ca1 Si1 88.33(7) 7 .
O2 Ca1 Si1 31.26(6) 4_565 .
O2 Ca1 Si1 163.38(6) 8_565 .
Si1 Ca1 Si1 104.38(4) 6_565 .
Si1 Ca1 Si1 93.93(4) 2_565 .
Si1 Ca1 Si1 133.09(4) 5 .
O3 Na2 O3 180.00(12) . 9
O3 Na2 O3 90.0 . 11
O3 Na2 O3 90.0 9 11
O3 Na2 O3 90.0 . 3
O3 Na2 O3 90.0 9 3
O3 Na2 O3 180.00(12) 11 3
O3 Na2 O1 128.34(5) . 9
O3 Na2 O1 51.66(5) 9 9
O3 Na2 O1 81.46(8) 11 9
O3 Na2 O1 98.54(8) 3 9
O3 Na2 O1 98.54(8) . 12
O3 Na2 O1 81.46(8) 9 12
O3 Na2 O1 128.34(5) 11 12
O3 Na2 O1 51.66(5) 3 12
O1 Na2 O1 53.62(6) 9 12
O3 Na2 O1 81.46(8) . 4
O3 Na2 O1 98.54(8) 9 4
O3 Na2 O1 51.66(5) 11 4
O3 Na2 O1 128.34(5) 3 4
O1 Na2 O1 126.38(6) 9 4
O1 Na2 O1 180.00(11) 12 4
O3 Na2 O1 81.46(8) . 11
O3 Na2 O1 98.54(8) 9 11
O3 Na2 O1 51.66(5) 11 11
O3 Na2 O1 128.34(5) 3 11
O1 Na2 O1 53.62(6) 9 11
O1 Na2 O1 79.26(10) 12 11
O1 Na2 O1 100.74(10) 4 11
O3 Na2 O1 98.54(8) . 3
O3 Na2 O1 81.46(8) 9 3
O3 Na2 O1 128.34(5) 11 3
O3 Na2 O1 51.66(5) 3 3
O1 Na2 O1 126.38(6) 9 3
O1 Na2 O1 100.74(10) 12 3
O1 Na2 O1 79.26(10) 4 3
O1 Na2 O1 180.00(13) 11 3
O3 Na2 O1 51.66(5) . 10
O3 Na2 O1 128.34(5) 9 10
O3 Na2 O1 98.54(8) 11 10
O3 Na2 O1 81.46(8) 3 10
O1 Na2 O1 79.26(10) 9 10
O1 Na2 O1 53.62(6) 12 10
O1 Na2 O1 126.38(6) 4 10
O1 Na2 O1 53.62(6) 11 10
O1 Na2 O1 126.38(6) 3 10
O3 Na2 O1 128.34(5) . 2
O3 Na2 O1 51.66(5) 9 2
O3 Na2 O1 81.46(8) 11 2
O3 Na2 O1 98.54(8) 3 2
O1 Na2 O1 100.74(10) 9 2
O1 Na2 O1 126.38(6) 12 2
O1 Na2 O1 53.62(6) 4 2
O1 Na2 O1 126.38(6) 11 2
O1 Na2 O1 53.62(6) 3 2
O1 Na2 O1 180.00(10) 10 2
O3 Na2 O1 51.66(5) . .
O3 Na2 O1 128.34(5) 9 .
O3 Na2 O1 98.54(8) 11 .
O3 Na2 O1 81.46(8) 3 .
O1 Na2 O1 180.00(6) 9 .
O1 Na2 O1 126.38(6) 12 .
O1 Na2 O1 53.62(6) 4 .
O1 Na2 O1 126.38(6) 11 .
O1 Na2 O1 53.62(6) 3 .
O1 Na2 O1 100.74(10) 10 .
O1 Na2 O1 79.26(10) 2 .
O3 Na2 Si1 153.447(18) . 9
O3 Na2 Si1 26.553(18) 9 9
O3 Na2 Si1 91.28(9) 11 9
O3 Na2 Si1 88.72(9) 3 9
O1 Na2 Si1 26.44(5) 9 9
O1 Na2 Si1 60.62(5) 12 9
O1 Na2 Si1 119.38(5) 4 9
O1 Na2 Si1 78.63(5) 11 9
O1 Na2 Si1 101.37(5) 3 9
O1 Na2 Si1 101.99(5) 10 9
O1 Na2 Si1 78.01(5) 2 9
O1 Na2 Si1 153.56(5) . 9
O3 Na2 Si1 26.553(18) . 10
O3 Na2 Si1 153.447(18) 9 10
O3 Na2 Si1 88.72(9) 11 10
O3 Na2 Si1 91.28(9) 3 10
O1 Na2 Si1 101.99(5) 9 10
O1 Na2 Si1 78.63(5) 12 10
O1 Na2 Si1 101.37(5) 4 10
O1 Na2 Si1 60.62(5) 11 10
O1 Na2 Si1 119.38(5) 3 10
O1 Na2 Si1 26.44(5) 10 10
O1 Na2 Si1 153.56(5) 2 10
O1 Na2 Si1 78.01(5) . 10
Si1 Na2 Si1 126.97(4) 9 10
O3 Na2 Si1 153.447(18) . 2
O3 Na2 Si1 26.553(18) 9 2
O3 Na2 Si1 91.28(9) 11 2
O3 Na2 Si1 88.72(9) 3 2
O1 Na2 Si1 78.01(5) 9 2
O1 Na2 Si1 101.37(5) 12 2
O1 Na2 Si1 78.63(5) 4 2
O1 Na2 Si1 119.38(5) 11 2
O1 Na2 Si1 60.62(5) 3 2
O1 Na2 Si1 153.56(5) 10 2
O1 Na2 Si1 26.44(5) 2 2
O1 Na2 Si1 101.99(5) . 2
Si1 Na2 Si1 53.03(4) 9 2
Si1 Na2 Si1 180.00(2) 10 2
O3 Na2 Si1 88.72(9) . 12
O3 Na2 Si1 91.28(9) 9 12
O3 Na2 Si1 153.447(18) 11 12
O3 Na2 Si1 26.553(18) 3 12
O1 Na2 Si1 78.63(5) 9 12
O1 Na2 Si1 26.44(5) 12 12
O1 Na2 Si1 153.56(5) 4 12
O1 Na2 Si1 101.99(5) 11 12
O1 Na2 Si1 78.01(5) 3 12
O1 Na2 Si1 60.62(5) 10 12
O1 Na2 Si1 119.38(5) 2 12
O1 Na2 Si1 101.37(5) . 12
Si1 Na2 Si1 78.502(14) 9 12
Si1 Na2 Si1 78.502(14) 10 12
Si1 Na2 Si1 101.498(14) 2 12
O1 Th1 O1 142.79(12) 2 7
O1 Th1 O1 141.77(12) 2 5
O1 Th1 O1 73.35(6) 7 5
O1 Th1 O1 73.35(6) 2 3
O1 Th1 O1 141.77(12) 7 3
O1 Th1 O1 77.09(13) 5 3
O1 Th1 O1 77.09(13) 2 8
O1 Th1 O1 115.28(14) 7 8
O1 Th1 O1 73.35(6) 5 8
O1 Th1 O1 77.73(13) 3 8
O1 Th1 O1 77.73(13) 2 6
O1 Th1 O1 73.35(6) 7 6
O1 Th1 O1 115.28(14) 5 6
O1 Th1 O1 142.79(12) 3 6
O1 Th1 O1 73.35(6) 8 6
O1 Th1 O1 73.35(6) 2 4
O1 Th1 O1 77.73(13) 7 4
O1 Th1 O1 142.79(12) 5 4
O1 Th1 O1 115.28(14) 3 4
O1 Th1 O1 141.77(12) 8 4
O1 Th1 O1 77.09(13) 6 4
O1 Th1 O1 115.28(14) 2 .
O1 Th1 O1 77.09(13) 7 .
O1 Th1 O1 77.73(13) 5 .
O1 Th1 O1 73.35(6) 3 .
O1 Th1 O1 142.79(12) 8 .
O1 Th1 O1 141.77(12) 6 .
O1 Th1 O1 73.35(6) 4 .
O1 Th1 Na2 57.64(7) 2 .
O1 Th1 Na2 122.36(7) 7 .
O1 Th1 Na2 122.36(7) 5 .
O1 Th1 Na2 57.64(7) 3 .
O1 Th1 Na2 122.36(7) 8 .
O1 Th1 Na2 122.36(7) 6 .
O1 Th1 Na2 57.64(7) 4 .
O1 Th1 Na2 57.64(7) . .
O1 Th1 Na2 122.36(7) 2 5
O1 Th1 Na2 57.64(7) 7 5
O1 Th1 Na2 57.64(7) 5 5
O1 Th1 Na2 122.36(7) 3 5
O1 Th1 Na2 57.64(7) 8 5
O1 Th1 Na2 57.64(7) 6 5
O1 Th1 Na2 122.36(7) 4 5
O1 Th1 Na2 122.36(7) . 5
Na2 Th1 Na2 180.0 . 5
O1 Th1 Ca1 38.86(7) 2 1_545
O1 Th1 Ca1 109.11(6) 7 1_545
O1 Th1 Ca1 141.14(7) 5 1_545
O1 Th1 Ca1 109.11(6) 3 1_545
O1 Th1 Ca1 70.89(6) 8 1_545
O1 Th1 Ca1 38.86(7) 6 1_545
O1 Th1 Ca1 70.89(6) 4 1_545
O1 Th1 Ca1 141.14(7) . 1_545
Na2 Th1 Ca1 90.0 . 1_545
Na2 Th1 Ca1 90.0 5 1_545
O1 Th1 Na1 109.11(6) 2 3_655
O1 Th1 Na1 38.86(7) 7 3_655
O1 Th1 Na1 109.11(6) 5 3_655
O1 Th1 Na1 141.14(7) 3 3_655
O1 Th1 Na1 141.14(7) 8 3_655
O1 Th1 Na1 70.89(6) 6 3_655
O1 Th1 Na1 38.86(7) 4 3_655
O1 Th1 Na1 70.89(6) . 3_655
Na2 Th1 Na1 90.0 . 3_655
Na2 Th1 Na1 90.0 5 3_655
Ca1 Th1 Na1 90.0 1_545 3_655
O1 Si1 O3 110.6(2) . .
O1 Si1 O2 113.69(15) . .
O3 Si1 O2 107.9(2) . .
O1 Si1 O2 105.68(16) . 4_565
O3 Si1 O2 110.5(2) . 4_565
O2 Si1 O2 108.5(2) . 4_565
O1 Si1 Ca1 48.40(10) . .
O3 Si1 Ca1 128.28(17) . .
O2 Si1 Ca1 123.79(11) . .
O2 Si1 Ca1 57.39(10) 4_565 .
O1 Si1 Na2 64.02(11) . .
O3 Si1 Na2 50.57(17) . .
O2 Si1 Na2 109.69(11) . .
O2 Si1 Na2 141.25(11) 4_565 .
Ca1 Si1 Na2 104.53(3) . .
Si1 O1 Th1 148.02(15) . .
Si1 O1 Ca1 102.46(13) . .
Th1 O1 Ca1 102.60(10) . .
Si1 O1 Na2 89.54(12) . .
Th1 O1 Na2 82.73(8) . .
Ca1 O1 Na2 142.08(10) . .
Si1 O2 Si1 147.2(2) . 3_655
Si1 O2 Na1 121.42(14) . 3_655
Si1 O2 Na1 91.34(12) 3_655 3_655
Si1 O2 Ca1 121.42(14) . 3_655
Si1 O2 Ca1 91.34(12) 3_655 3_655
Na1 O2 Ca1 0.0 3_655 3_655
Si1 O2 Na2 49.75(9) . .
Si1 O2 Na2 132.64(13) 3_655 .
Na1 O2 Na2 94.86(7) 3_655 .
Ca1 O2 Na2 94.86(7) 3_655 .
Si1 O3 Si1 153.6(4) . 10
Si1 O3 Na2 102.88(18) . .
Si1 O3 Na2 102.88(18) 10 .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Ca1 O1 2.410(3) .
Ca1 O1 2.410(3) 6_565
Ca1 O1 2.410(3) 5
Ca1 O1 2.410(3) 2_565
Ca1 O2 2.652(3) 3
Ca1 O2 2.652(3) 7
Ca1 O2 2.652(3) 4_565
Ca1 O2 2.652(3) 8_565
Ca1 Si1 3.1470(11) 6_565
Ca1 Si1 3.1470(11) 2_565
Ca1 Si1 3.1470(11) 5
Ca1 Si1 3.1470(11) .
Na2 O3 2.793(5) .
Na2 O3 2.793(5) 9
Na2 O3 2.793(5) 11
Na2 O3 2.793(5) 3
Na2 O1 3.169(3) 9
Na2 O1 3.169(3) 12
Na2 O1 3.169(3) 4
Na2 O1 3.169(3) 11
Na2 O1 3.169(3) 3
Na2 O1 3.169(3) 10
Na2 O1 3.169(3) 2
Na2 O1 3.169(3) .
Na2 Si1 3.5252(12) 9
Na2 Si1 3.5252(12) 10
Na2 Si1 3.5252(12) 2
Na2 Si1 3.5252(12) 12
Th1 O1 2.393(3) 2
Th1 O1 2.393(3) 7
Th1 O1 2.393(3) 5
Th1 O1 2.393(3) 3
Th1 O1 2.393(3) 8
Th1 O1 2.393(3) 6
Th1 O1 2.393(3) 4
Th1 O1 2.393(3) .
Th1 Na2 3.7215(10) 5
Th1 Ca1 3.7483(10) 1_545
Th1 Na1 3.7483(10) 3_655
Si1 O1 1.570(3) .
Si1 O3 1.6165(15) .
Si1 O2 1.622(3) .
Si1 O2 1.634(3) 4_565
O2 Si1 1.634(3) 3_655
O2 Na1 2.652(3) 3_655
O2 Ca1 2.652(3) 3_655
O3 Si1 1.6165(15) 10
